#------------------------------------------------------------------------------
#$Date: 2025-10-06 11:42:37 +0200 (Mon 06 de Oct de 2025) $
#$Revision: 302676 $
#$URL: svn://www.crystallography.net/cod/cif/7/71/91/7719184.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7719184
loop_
_publ_author_name
'Rahman, Salina'
'Ghosh, Kowsik'
'Ovchinnikov, Alexander'
'Nandakumar, Anirudh'
'Chan, Candace K.'
'Bobev, Svilen'
_publ_section_title
;
 On the structure of heptalithium distannide: Li₇Sn₂
 or Li₇₋ₓSn₂ (0.3 < x < 0.5).
;
_journal_issue                   34
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              12859
_journal_page_last               12867
_journal_paper_doi               10.1039/d5dt01022e
_journal_volume                  54
_journal_year                    2025
_chemical_formula_sum            'Li6.5 Sn2'
_chemical_formula_weight         282.49
_space_group_IT_number           65
_space_group_name_Hall           '-C 2 2'
_space_group_name_H-M_alt        'C m m m'
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_H-M   'C m m m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2025-04-16 deposited with the CCDC.	2025-07-23 downloaded from the CCDC.
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   9.8105(10)
_cell_length_b                   13.8521(14)
_cell_length_c                   4.7272(5)
_cell_measurement_reflns_used    1112
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      30.47
_cell_measurement_theta_min      2.54
_cell_volume                     642.41(11)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      200(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0397
_diffrn_reflns_av_sigmaI/netI    0.0351
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_limit_l_min       -6
_diffrn_reflns_number            2757
_diffrn_reflns_theta_full        30.63
_diffrn_reflns_theta_max         30.63
_diffrn_reflns_theta_min         2.54
_exptl_absorpt_coefficient_mu    7.618
_exptl_absorpt_correction_T_max  0.5774
_exptl_absorpt_correction_T_min  0.3393
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    2.921
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       irregular
_exptl_crystal_F_000             478
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.08
_refine_diff_density_max         1.392
_refine_diff_density_min         -1.311
_refine_diff_density_rms         0.225
_refine_ls_extinction_coef       0.0033(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.064
_refine_ls_matrix_type           full
_refine_ls_number_parameters     21
_refine_ls_number_reflns         593
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.064
_refine_ls_R_factor_all          0.0351
_refine_ls_R_factor_gt           0.0257
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0274P)²+0.3498P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0564
_refine_ls_wR_factor_ref         0.0591
_reflns_number_gt                493
_reflns_number_total             593
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            d5dt01022e2.cif
_cod_data_source_block           final_CCDC7
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Orthorhombic' was changed
to 'orthorhombic' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 8170 2020-07-09 18:12:32Z antanas 

 Adding full bibliography for 7719177--7719189.cif.
;
_cod_original_sg_symbol_H-M      Cmmm
_cod_original_formula_sum        'Li6.50 Sn2'
_cod_database_code               7719184
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Sn1 Sn 0.34736(4) 0.0000 0.0000 0.01150(17) Uani 1 4 d S . .
Sn2 Sn 0.0000 0.18787(3) 0.5000 0.01132(17) Uani 1 4 d S . .
Li1 Li 0.3092(11) 0.1566(8) 0.5000 0.027(2) Uiso 1 2 d S . .
Li2 Li 0.1475(12) 0.1458(10) 0.0000 0.040(3) Uiso 1 2 d S . .
Li3 Li 0.1458(15) 0.0000 0.5000 0.031(4) Uiso 1 4 d S . .
Li4 Li 0.0000 0.3200(11) 0.0000 0.028(3) Uiso 1 4 d S . .
Li5 Li 0.5000 0.0000 0.5000 0.038(6) Uiso 1 8 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sn Sn -0.6537 1.4246 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Li5 Sn1 Li5 115.287(17) . 1_554 ?
Li5 Sn1 Li2 111.89(11) . 11 ?
Li5 Sn1 Li2 111.89(11) 1_554 11 ?
Li5 Sn1 Li2 111.89(11) . . ?
Li5 Sn1 Li2 111.89(11) 1_554 . ?
Li2 Sn1 Li2 91.7(5) 11 . ?
Li5 Sn1 Li4 74.01(7) . 13 ?
Li5 Sn1 Li4 74.01(7) 1_554 13 ?
Li2 Sn1 Li4 166.8(3) 11 13 ?
Li2 Sn1 Li4 75.1(3) . 13 ?
Li5 Sn1 Li4 74.01(7) . 5_545 ?
Li5 Sn1 Li4 74.01(7) 1_554 5_545 ?
Li2 Sn1 Li4 75.1(3) 11 5_545 ?
Li2 Sn1 Li4 166.8(3) . 5_545 ?
Li4 Sn1 Li4 118.0(3) 13 5_545 ?
Li5 Sn1 Sn1 57.644(8) . 9_655 ?
Li5 Sn1 Sn1 57.644(8) 1_554 9_655 ?
Li2 Sn1 Sn1 134.1(3) 11 9_655 ?
Li2 Sn1 Sn1 134.1(3) . 9_655 ?
Li4 Sn1 Sn1 59.02(15) 13 9_655 ?
Li4 Sn1 Sn1 59.02(15) 5_545 9_655 ?
Li5 Sn1 Li3 172.4(2) . 1_554 ?
Li5 Sn1 Li3 72.3(2) 1_554 1_554 ?
Li2 Sn1 Li3 63.45(19) 11 1_554 ?
Li2 Sn1 Li3 63.45(19) . 1_554 ?
Li4 Sn1 Li3 109.29(13) 13 1_554 ?
Li4 Sn1 Li3 109.29(13) 5_545 1_554 ?
Sn1 Sn1 Li3 129.9(2) 9_655 1_554 ?
Li5 Sn1 Li3 72.3(2) . . ?
Li5 Sn1 Li3 172.4(2) 1_554 . ?
Li2 Sn1 Li3 63.45(19) 11 . ?
Li2 Sn1 Li3 63.45(19) . . ?
Li4 Sn1 Li3 109.29(13) 13 . ?
Li4 Sn1 Li3 109.29(13) 5_545 . ?
Sn1 Sn1 Li3 129.9(2) 9_655 . ?
Li3 Sn1 Li3 100.2(4) 1_554 . ?
Li5 Sn1 Li1 132.87(17) . 11_554 ?
Li5 Sn1 Li1 56.21(17) 1_554 11_554 ?
Li2 Sn1 Li1 55.8(2) 11 11_554 ?
Li2 Sn1 Li1 113.6(2) . 11_554 ?
Li4 Sn1 Li1 129.45(17) 13 11_554 ?
Li4 Sn1 Li1 58.94(18) 5_545 11_554 ?
Sn1 Sn1 Li1 96.66(19) 9_655 11_554 ?
Li3 Sn1 Li1 50.5(2) 1_554 11_554 ?
Li3 Sn1 Li1 119.1(2) . 11_554 ?
Li5 Sn1 Li1 132.87(17) . 1_554 ?
Li5 Sn1 Li1 56.21(17) 1_554 1_554 ?
Li2 Sn1 Li1 113.6(2) 11 1_554 ?
Li2 Sn1 Li1 55.8(2) . 1_554 ?
Li4 Sn1 Li1 58.94(18) 13 1_554 ?
Li4 Sn1 Li1 129.45(17) 5_545 1_554 ?
Sn1 Sn1 Li1 96.66(19) 9_655 1_554 ?
Li3 Sn1 Li1 50.5(2) 1_554 1_554 ?
Li3 Sn1 Li1 119.1(2) . 1_554 ?
Li1 Sn1 Li1 84.4(3) 11_554 1_554 ?
Li5 Sn1 Li1 56.21(17) . 11 ?
Li5 Sn1 Li1 132.87(17) 1_554 11 ?
Li2 Sn1 Li1 55.8(2) 11 11 ?
Li2 Sn1 Li1 113.6(2) . 11 ?
Li4 Sn1 Li1 129.45(17) 13 11 ?
Li4 Sn1 Li1 58.94(18) 5_545 11 ?
Sn1 Sn1 Li1 96.66(19) 9_655 11 ?
Li3 Sn1 Li1 119.1(2) 1_554 11 ?
Li3 Sn1 Li1 50.5(2) . 11 ?
Li1 Sn1 Li1 94.1(3) 11_554 11 ?
Li1 Sn1 Li1 166.7(4) 1_554 11 ?
Li2 Sn2 Li2 61.5(4) . 3 ?
Li2 Sn2 Li2 113.1(4) . 1_556 ?
Li2 Sn2 Li2 156.2(5) 3 1_556 ?
Li2 Sn2 Li2 156.2(5) . 3_556 ?
Li2 Sn2 Li2 113.1(4) 3 3_556 ?
Li2 Sn2 Li2 61.5(4) 1_556 3_556 ?
Li2 Sn2 Li1 79.6(3) . 13_556 ?
Li2 Sn2 Li1 119.4(2) 3 13_556 ?
Li2 Sn2 Li1 79.6(3) 1_556 13_556 ?
Li2 Sn2 Li1 119.4(3) 3_556 13_556 ?
Li2 Sn2 Li1 119.4(2) . 15_455 ?
Li2 Sn2 Li1 79.6(3) 3 15_455 ?
Li2 Sn2 Li1 119.4(2) 1_556 15_455 ?
Li2 Sn2 Li1 79.6(3) 3_556 15_455 ?
Li1 Sn2 Li1 82.0(5) 13_556 15_455 ?
Li2 Sn2 Li3 64.8(3) . . ?
Li2 Sn2 Li3 93.8(3) 3 . ?
Li2 Sn2 Li3 64.8(3) 1_556 . ?
Li2 Sn2 Li3 93.8(3) 3_556 . ?
Li1 Sn2 Li3 110.2(3) 13_556 . ?
Li1 Sn2 Li3 167.8(4) 15_455 . ?
Li2 Sn2 Li3 93.8(3) . 9_556 ?
Li2 Sn2 Li3 64.8(3) 3 9_556 ?
Li2 Sn2 Li3 93.8(3) 1_556 9_556 ?
Li2 Sn2 Li3 64.8(3) 3_556 9_556 ?
Li1 Sn2 Li3 167.8(3) 13_556 9_556 ?
Li1 Sn2 Li3 110.2(3) 15_455 9_556 ?
Li3 Sn2 Li3 57.6(5) . 9_556 ?
Li2 Sn2 Li4 141.8(3) . 1_556 ?
Li2 Sn2 Li4 141.8(3) 3 1_556 ?
Li2 Sn2 Li4 57.7(3) 1_556 1_556 ?
Li2 Sn2 Li4 57.7(3) 3_556 1_556 ?
Li1 Sn2 Li4 62.47(18) 13_556 1_556 ?
Li1 Sn2 Li4 62.47(18) 15_455 1_556 ?
Li3 Sn2 Li4 122.4(2) . 1_556 ?
Li3 Sn2 Li4 122.4(2) 9_556 1_556 ?
Li2 Sn2 Li4 57.7(3) . . ?
Li2 Sn2 Li4 57.7(3) 3 . ?
Li2 Sn2 Li4 141.8(3) 1_556 . ?
Li2 Sn2 Li4 141.8(3) 3_556 . ?
Li1 Sn2 Li4 62.47(18) 13_556 . ?
Li1 Sn2 Li4 62.47(18) 15_455 . ?
Li3 Sn2 Li4 122.4(2) . . ?
Li3 Sn2 Li4 122.4(2) 9_556 . ?
Li4 Sn2 Li4 104.5(4) 1_556 . ?
Li2 Sn2 Li1 57.7(2) . . ?
Li2 Sn2 Li1 118.5(2) 3 . ?
Li2 Sn2 Li1 57.7(2) 1_556 . ?
Li2 Sn2 Li1 118.5(2) 3_556 . ?
Li1 Sn2 Li1 57.2(4) 13_556 . ?
Li1 Sn2 Li1 139.1(2) 15_455 . ?
Li3 Sn2 Li1 53.1(3) . . ?
Li3 Sn2 Li1 110.7(3) 9_556 . ?
Li4 Sn2 Li1 94.97(13) 1_556 . ?
Li4 Sn2 Li1 94.97(13) . . ?
Li2 Sn2 Li1 118.5(2) . 3_556 ?
Li2 Sn2 Li1 57.7(2) 3 3_556 ?
Li2 Sn2 Li1 118.5(2) 1_556 3_556 ?
Li2 Sn2 Li1 57.7(2) 3_556 3_556 ?
Li1 Sn2 Li1 139.1(2) 13_556 3_556 ?
Li1 Sn2 Li1 57.2(4) 15_455 3_556 ?
Li3 Sn2 Li1 110.7(3) . 3_556 ?
Li3 Sn2 Li1 53.1(3) 9_556 3_556 ?
Li4 Sn2 Li1 94.97(13) 1_556 3_556 ?
Li4 Sn2 Li1 94.97(13) . 3_556 ?
Li1 Sn2 Li1 163.7(4) . 3_556 ?
Li3 Li1 Li1 119.4(6) . 13_556 ?
Li3 Li1 Sn2 175.5(5) . 13_556 ?
Li1 Li1 Sn2 65.1(4) 13_556 13_556 ?
Li3 Li1 Li2 68.1(4) . . ?
Li1 Li1 Li2 79.6(4) 13_556 . ?
Sn2 Li1 Li2 113.9(4) 13_556 . ?
Li3 Li1 Li2 68.1(4) . 1_556 ?
Li1 Li1 Li2 79.6(4) 13_556 1_556 ?
Sn2 Li1 Li2 113.9(4) 13_556 1_556 ?
Li2 Li1 Li2 112.1(5) . 1_556 ?
Li3 Li1 Li5 77.3(4) . . ?
Li1 Li1 Li5 163.4(6) 13_556 . ?
Sn2 Li1 Li5 98.2(3) 13_556 . ?
Li2 Li1 Li5 108.9(4) . . ?
Li2 Li1 Li5 108.9(4) 1_556 . ?
Li3 Li1 Li4 116.9(4) . 13_556 ?
Li1 Li1 Li4 98.9(5) 13_556 13_556 ?
Sn2 Li1 Li4 60.9(3) 13_556 13_556 ?
Li2 Li1 Li4 174.5(4) . 13_556 ?
Li2 Li1 Li4 72.7(2) 1_556 13_556 ?
Li5 Li1 Li4 71.2(3) . 13_556 ?
Li3 Li1 Li4 116.9(4) . 13 ?
Li1 Li1 Li4 98.9(5) 13_556 13 ?
Sn2 Li1 Li4 60.9(3) 13_556 13 ?
Li2 Li1 Li4 72.7(2) . 13 ?
Li2 Li1 Li4 174.5(4) 1_556 13 ?
Li5 Li1 Li4 71.2(3) . 13 ?
Li4 Li1 Li4 102.4(3) 13_556 13 ?
Li3 Li1 Sn2 61.7(3) . . ?
Li1 Li1 Sn2 57.7(4) 13_556 . ?
Sn2 Li1 Sn2 122.8(4) 13_556 . ?
Li2 Li1 Sn2 57.1(3) . . ?
Li2 Li1 Sn2 57.1(3) 1_556 . ?
Li5 Li1 Sn2 138.9(4) . . ?
Li4 Li1 Sn2 126.6(2) 13_556 . ?
Li4 Li1 Sn2 126.6(2) 13 . ?
Li3 Li1 Sn1 61.9(2) . . ?
Li1 Li1 Sn1 131.3(2) 13_556 . ?
Sn2 Li1 Sn1 115.5(2) 13_556 . ?
Li2 Li1 Sn1 54.7(3) . . ?
Li2 Li1 Sn1 129.5(5) 1_556 . ?
Li5 Li1 Sn1 54.26(17) . . ?
Li4 Li1 Sn1 124.8(4) 13_556 . ?
Li4 Li1 Sn1 55.2(3) 13 . ?
Sn2 Li1 Sn1 102.1(2) . . ?
Li3 Li1 Sn1 61.9(2) . 1_556 ?
Li1 Li1 Sn1 131.3(2) 13_556 1_556 ?
Sn2 Li1 Sn1 115.5(2) 13_556 1_556 ?
Li2 Li1 Sn1 129.5(5) . 1_556 ?
Li2 Li1 Sn1 54.7(3) 1_556 1_556 ?
Li5 Li1 Sn1 54.26(17) . 1_556 ?
Li4 Li1 Sn1 55.2(3) 13_556 1_556 ?
Li4 Li1 Sn1 124.8(4) 13 1_556 ?
Sn2 Li1 Sn1 102.1(2) . 1_556 ?
Sn1 Li1 Sn1 94.1(3) . 1_556 ?
Li4 Li2 Sn1 166.8(5) . . ?
Li4 Li2 Sn2 63.9(2) . 1_554 ?
Sn1 Li2 Sn2 120.2(3) . 1_554 ?
Li4 Li2 Sn2 63.9(2) . . ?
Sn1 Li2 Sn2 120.2(3) . . ?
Sn2 Li2 Sn2 113.1(4) 1_554 . ?
Li4 Li2 Li1 104.0(4) . . ?
Sn1 Li2 Li1 69.5(3) . . ?
Sn2 Li2 Li1 164.9(6) 1_554 . ?
Sn2 Li2 Li1 65.3(2) . . ?
Li4 Li2 Li1 104.0(4) . 1_554 ?
Sn1 Li2 Li1 69.5(3) . 1_554 ?
Sn2 Li2 Li1 65.26(19) 1_554 1_554 ?
Sn2 Li2 Li1 164.9(6) . 1_554 ?
Li1 Li2 Li1 112.1(5) . 1_554 ?
Li4 Li2 Li2 59.0(3) . 3 ?
Sn1 Li2 Li2 134.1(3) . 3 ?
Sn2 Li2 Li2 59.3(2) 1_554 3 ?
Sn2 Li2 Li2 59.3(2) . 3 ?
Li1 Li2 Li2 123.8(3) . 3 ?
Li1 Li2 Li2 123.8(3) 1_554 3 ?
Li4 Li2 Li3 123.7(3) . 1_554 ?
Sn1 Li2 Li3 62.5(3) . 1_554 ?
Sn2 Li2 Li3 59.76(18) 1_554 1_554 ?
Sn2 Li2 Li3 139.9(5) . 1_554 ?
Li1 Li2 Li3 131.9(6) . 1_554 ?
Li1 Li2 Li3 53.6(3) 1_554 1_554 ?
Li2 Li2 Li3 89.7(3) 3 1_554 ?
Li4 Li2 Li3 123.7(3) . . ?
Sn1 Li2 Li3 62.5(3) . . ?
Sn2 Li2 Li3 139.9(5) 1_554 . ?
Sn2 Li2 Li3 59.76(18) . . ?
Li1 Li2 Li3 53.6(3) . . ?
Li1 Li2 Li3 131.9(6) 1_554 . ?
Li2 Li2 Li3 89.7(3) 3 . ?
Li3 Li2 Li3 99.0(4) 1_554 . ?
Li4 Li2 Li4 113.1(4) . 13 ?
Sn1 Li2 Li4 53.7(3) . 13 ?
Sn2 Li2 Li4 118.6(3) 1_554 13 ?
Sn2 Li2 Li4 118.6(3) . 13 ?
Li1 Li2 Li4 56.1(2) . 13 ?
Li1 Li2 Li4 56.1(2) 1_554 13 ?
Li2 Li2 Li4 172.2(3) 3 13 ?
Li3 Li2 Li4 95.4(4) 1_554 13 ?
Li3 Li2 Li4 95.4(4) . 13 ?
Li4 Li2 Li2 65.8(4) . 13 ?
Sn1 Li2 Li2 101.0(5) . 13 ?
Sn2 Li2 Li2 97.1(4) 1_554 13 ?
Sn2 Li2 Li2 97.1(4) . 13 ?
Li1 Li2 Li2 68.8(3) . 13 ?
Li1 Li2 Li2 68.8(3) 1_554 13 ?
Li2 Li2 Li2 124.8(4) 3 13 ?
Li3 Li2 Li2 122.4(3) 1_554 13 ?
Li3 Li2 Li2 122.4(3) . 13 ?
Li4 Li2 Li2 47.3(4) 13 13 ?
Li1 Li3 Li1 107.1(7) 11 . ?
Li1 Li3 Li3 126.5(3) 11 9_556 ?
Li1 Li3 Li3 126.5(3) . 9_556 ?
Li1 Li3 Sn2 65.3(2) 11 9_556 ?
Li1 Li3 Sn2 172.3(5) . 9_556 ?
Li3 Li3 Sn2 61.2(3) 9_556 9_556 ?
Li1 Li3 Sn2 172.3(5) 11 . ?
Li1 Li3 Sn2 65.3(2) . . ?
Li3 Li3 Sn2 61.2(3) 9_556 . ?
Sn2 Li3 Sn2 122.4(5) 9_556 . ?
Li1 Li3 Sn1 67.6(3) 11 1_556 ?
Li1 Li3 Sn1 67.6(3) . 1_556 ?
Li3 Li3 Sn1 129.9(2) 9_556 1_556 ?
Sn2 Li3 Sn1 108.00(7) 9_556 1_556 ?
Sn2 Li3 Sn1 108.00(7) . 1_556 ?
Li1 Li3 Sn1 67.6(3) 11 . ?
Li1 Li3 Sn1 67.6(3) . . ?
Li3 Li3 Sn1 129.9(2) 9_556 . ?
Sn2 Li3 Sn1 108.00(7) 9_556 . ?
Sn2 Li3 Sn1 108.00(7) . . ?
Sn1 Li3 Sn1 100.2(4) 1_556 . ?
Li1 Li3 Li2 58.3(2) 11 11 ?
Li1 Li3 Li2 121.3(4) . 11 ?
Li3 Li3 Li2 90.3(3) 9_556 11 ?
Sn2 Li3 Li2 55.5(2) 9_556 11 ?
Sn2 Li3 Li2 124.9(3) . 11 ?
Sn1 Li3 Li2 125.4(4) 1_556 11 ?
Sn1 Li3 Li2 54.1(2) . 11 ?
Li1 Li3 Li2 121.3(4) 11 1_556 ?
Li1 Li3 Li2 58.3(2) . 1_556 ?
Li3 Li3 Li2 90.3(3) 9_556 1_556 ?
Sn2 Li3 Li2 124.9(3) 9_556 1_556 ?
Sn2 Li3 Li2 55.5(2) . 1_556 ?
Sn1 Li3 Li2 54.1(2) 1_556 1_556 ?
Sn1 Li3 Li2 125.4(4) . 1_556 ?
Li2 Li3 Li2 179.4(7) 11 1_556 ?
Li1 Li3 Li2 58.3(2) 11 11_556 ?
Li1 Li3 Li2 121.3(4) . 11_556 ?
Li3 Li3 Li2 90.3(3) 9_556 11_556 ?
Sn2 Li3 Li2 55.5(2) 9_556 11_556 ?
Sn2 Li3 Li2 124.9(3) . 11_556 ?
Sn1 Li3 Li2 54.1(2) 1_556 11_556 ?
Sn1 Li3 Li2 125.4(4) . 11_556 ?
Li2 Li3 Li2 99.0(4) 11 11_556 ?
Li2 Li3 Li2 81.0(4) 1_556 11_556 ?
Li1 Li3 Li2 121.3(4) 11 . ?
Li1 Li3 Li2 58.3(2) . . ?
Li3 Li3 Li2 90.3(3) 9_556 . ?
Sn2 Li3 Li2 124.9(3) 9_556 . ?
Sn2 Li3 Li2 55.5(2) . . ?
Sn1 Li3 Li2 125.4(4) 1_556 . ?
Sn1 Li3 Li2 54.1(2) . . ?
Li2 Li3 Li2 81.0(4) 11 . ?
Li2 Li3 Li2 99.0(4) 1_556 . ?
Li2 Li3 Li2 179.4(7) 11_556 . ?
Li1 Li3 Li5 53.5(3) 11 . ?
Li1 Li3 Li5 53.5(3) . . ?
Li3 Li3 Li5 180.0 9_556 . ?
Sn2 Li3 Li5 118.8(3) 9_556 . ?
Sn2 Li3 Li5 118.8(3) . . ?
Sn1 Li3 Li5 50.1(2) 1_556 . ?
Sn1 Li3 Li5 50.1(2) . . ?
Li2 Li3 Li5 89.7(3) 11 . ?
Li2 Li3 Li5 89.7(3) 1_556 . ?
Li2 Li3 Li5 89.7(3) 11_556 . ?
Li2 Li3 Li5 89.7(3) . . ?
Li2 Li4 Li2 61.9(6) . 3 ?
Li2 Li4 Sn1 118.1(3) . 13 ?
Li2 Li4 Sn1 180.0(4) 3 13 ?
Li2 Li4 Sn1 180.0(4) . 5_455 ?
Li2 Li4 Sn1 118.1(3) 3 5_455 ?
Sn1 Li4 Sn1 62.0(3) 13 5_455 ?
Li2 Li4 Sn2 58.3(2) . . ?
Li2 Li4 Sn2 58.3(2) 3 . ?
Sn1 Li4 Sn2 121.66(12) 13 . ?
Sn1 Li4 Sn2 121.66(12) 5_455 . ?
Li2 Li4 Sn2 58.3(2) . 1_554 ?
Li2 Li4 Sn2 58.3(2) 3 1_554 ?
Sn1 Li4 Sn2 121.66(12) 13 1_554 ?
Sn1 Li4 Sn2 121.66(12) 5_455 1_554 ?
Sn2 Li4 Sn2 104.5(4) . 1_554 ?
Li2 Li4 Li1 77.0(3) . 13_556 ?
Li2 Li4 Li1 114.2(4) 3 13_556 ?
Sn1 Li4 Li1 65.8(3) 13 13_556 ?
Sn1 Li4 Li1 103.1(4) 5_455 13_556 ?
Sn2 Li4 Li1 56.6(2) . 13_556 ?
Sn2 Li4 Li1 133.0(4) 1_554 13_556 ?
Li2 Li4 Li1 114.2(4) . 15_454 ?
Li2 Li4 Li1 77.0(3) 3 15_454 ?
Sn1 Li4 Li1 103.1(4) 13 15_454 ?
Sn1 Li4 Li1 65.8(3) 5_455 15_454 ?
Sn2 Li4 Li1 133.0(4) . 15_454 ?
Sn2 Li4 Li1 56.6(2) 1_554 15_454 ?
Li1 Li4 Li1 167.7(7) 13_556 15_454 ?
Li2 Li4 Li1 77.0(3) . 13 ?
Li2 Li4 Li1 114.2(4) 3 13 ?
Sn1 Li4 Li1 65.8(3) 13 13 ?
Sn1 Li4 Li1 103.1(4) 5_455 13 ?
Sn2 Li4 Li1 133.0(4) . 13 ?
Sn2 Li4 Li1 56.6(2) 1_554 13 ?
Li1 Li4 Li1 102.4(3) 13_556 13 ?
Li1 Li4 Li1 76.2(3) 15_454 13 ?
Li2 Li4 Li1 114.2(4) . 15_455 ?
Li2 Li4 Li1 77.0(3) 3 15_455 ?
Sn1 Li4 Li1 103.1(4) 13 15_455 ?
Sn1 Li4 Li1 65.8(3) 5_455 15_455 ?
Sn2 Li4 Li1 56.6(2) . 15_455 ?
Sn2 Li4 Li1 133.0(4) 1_554 15_455 ?
Li1 Li4 Li1 76.2(3) 13_556 15_455 ?
Li1 Li4 Li1 102.4(3) 15_454 15_455 ?
Li1 Li4 Li1 167.7(7) 13 15_455 ?
Li2 Li4 Li5 128.49(14) . 5_455 ?
Li2 Li4 Li5 128.49(14) 3 5_455 ?
Sn1 Li4 Li5 51.5(2) 13 5_455 ?
Sn1 Li4 Li5 51.5(2) 5_455 5_455 ?
Sn2 Li4 Li5 84.28(5) . 5_455 ?
Sn2 Li4 Li5 171.2(4) 1_554 5_455 ?
Li1 Li4 Li5 52.1(2) 13_556 5_455 ?
Li1 Li4 Li5 117.3(4) 15_454 5_455 ?
Li1 Li4 Li5 117.3(4) 13 5_455 ?
Li1 Li4 Li5 52.1(2) 15_455 5_455 ?
Li2 Li4 Li5 128.49(14) . 5_454 ?
Li2 Li4 Li5 128.49(14) 3 5_454 ?
Sn1 Li4 Li5 51.5(2) 13 5_454 ?
Sn1 Li4 Li5 51.5(2) 5_455 5_454 ?
Sn2 Li4 Li5 171.2(4) . 5_454 ?
Sn2 Li4 Li5 84.28(5) 1_554 5_454 ?
Li1 Li4 Li5 117.3(4) 13_556 5_454 ?
Li1 Li4 Li5 52.1(2) 15_454 5_454 ?
Li1 Li4 Li5 52.1(2) 13 5_454 ?
Li1 Li4 Li5 117.3(4) 15_455 5_454 ?
Li5 Li4 Li5 86.9(3) 5_455 5_454 ?
Sn1 Li5 Sn1 180.0 . 9_656 ?
Sn1 Li5 Sn1 64.713(17) . 9_655 ?
Sn1 Li5 Sn1 115.287(17) 9_656 9_655 ?
Sn1 Li5 Sn1 115.287(17) . 1_556 ?
Sn1 Li5 Sn1 64.713(17) 9_656 1_556 ?
Sn1 Li5 Sn1 180.000(15) 9_655 1_556 ?
Sn1 Li5 Li1 69.53(9) . 11 ?
Sn1 Li5 Li1 110.47(9) 9_656 11 ?
Sn1 Li5 Li1 110.47(9) 9_655 11 ?
Sn1 Li5 Li1 69.53(9) 1_556 11 ?
Sn1 Li5 Li1 110.47(9) . 3_656 ?
Sn1 Li5 Li1 69.53(9) 9_656 3_656 ?
Sn1 Li5 Li1 69.53(9) 9_655 3_656 ?
Sn1 Li5 Li1 110.47(9) 1_556 3_656 ?
Li1 Li5 Li1 180.0(3) 11 3_656 ?
Sn1 Li5 Li1 110.47(9) . 9_656 ?
Sn1 Li5 Li1 69.53(9) 9_656 9_656 ?
Sn1 Li5 Li1 69.53(9) 9_655 9_656 ?
Sn1 Li5 Li1 110.47(9) 1_556 9_656 ?
Li1 Li5 Li1 81.6(4) 11 9_656 ?
Li1 Li5 Li1 98.4(4) 3_656 9_656 ?
Sn1 Li5 Li1 69.53(9) . . ?
Sn1 Li5 Li1 110.47(9) 9_656 . ?
Sn1 Li5 Li1 110.47(9) 9_655 . ?
Sn1 Li5 Li1 69.53(9) 1_556 . ?
Li1 Li5 Li1 98.4(4) 11 . ?
Li1 Li5 Li1 81.6(4) 3_656 . ?
Li1 Li5 Li1 180.000(1) 9_656 . ?
Sn1 Li5 Li4 125.53(13) . 13_556 ?
Sn1 Li5 Li4 54.47(13) 9_656 13_556 ?
Sn1 Li5 Li4 125.53(13) 9_655 13_556 ?
Sn1 Li5 Li4 54.47(13) 1_556 13_556 ?
Li1 Li5 Li4 123.33(16) 11 13_556 ?
Li1 Li5 Li4 56.67(16) 3_656 13_556 ?
Li1 Li5 Li4 123.33(16) 9_656 13_556 ?
Li1 Li5 Li4 56.67(16) . 13_556 ?
Sn1 Li5 Li4 54.47(13) . 5_545 ?
Sn1 Li5 Li4 125.53(13) 9_656 5_545 ?
Sn1 Li5 Li4 54.47(13) 9_655 5_545 ?
Sn1 Li5 Li4 125.53(13) 1_556 5_545 ?
Li1 Li5 Li4 56.67(16) 11 5_545 ?
Li1 Li5 Li4 123.33(16) 3_656 5_545 ?
Li1 Li5 Li4 56.67(16) 9_656 5_545 ?
Li1 Li5 Li4 123.33(16) . 5_545 ?
Li4 Li5 Li4 180.0 13_556 5_545 ?
Sn1 Li5 Li4 54.47(13) . 13 ?
Sn1 Li5 Li4 125.53(13) 9_656 13 ?
Sn1 Li5 Li4 54.47(13) 9_655 13 ?
Sn1 Li5 Li4 125.53(13) 1_556 13 ?
Li1 Li5 Li4 123.33(16) 11 13 ?
Li1 Li5 Li4 56.67(16) 3_656 13 ?
Li1 Li5 Li4 123.33(16) 9_656 13 ?
Li1 Li5 Li4 56.67(16) . 13 ?
Li4 Li5 Li4 86.9(3) 13_556 13 ?
Li4 Li5 Li4 93.1(3) 5_545 13 ?
Sn1 Li5 Li4 125.53(13) . 5_546 ?
Sn1 Li5 Li4 54.47(13) 9_656 5_546 ?
Sn1 Li5 Li4 125.53(13) 9_655 5_546 ?
Sn1 Li5 Li4 54.47(13) 1_556 5_546 ?
Li1 Li5 Li4 56.67(16) 11 5_546 ?
Li1 Li5 Li4 123.33(16) 3_656 5_546 ?
Li1 Li5 Li4 56.67(16) 9_656 5_546 ?
Li1 Li5 Li4 123.33(16) . 5_546 ?
Li4 Li5 Li4 93.1(3) 13_556 5_546 ?
Li4 Li5 Li4 86.9(3) 5_545 5_546 ?
Li4 Li5 Li4 180.0(3) 13 5_546 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Sn1 Li5 2.7980(3) . ?
Sn1 Li5 2.7980(3) 1_554 ?
Sn1 Li2 2.814(13) 11 ?
Sn1 Li2 2.814(13) . ?
Sn1 Li4 2.909(12) 13 ?
Sn1 Li4 2.909(12) 5_545 ?
Sn1 Sn1 2.9949(9) 9_655 ?
Sn1 Li3 3.082(10) 1_554 ?
Sn1 Li3 3.082(10) . ?
Sn1 Li1 3.230(8) 11_554 ?
Sn1 Li1 3.230(8) 1_554 ?
Sn1 Li1 3.230(8) 11 ?
Sn2 Li2 2.832(7) . ?
Sn2 Li2 2.832(7) 3 ?
Sn2 Li2 2.832(7) 1_556 ?
Sn2 Li2 2.832(7) 3_556 ?
Sn2 Li1 2.854(11) 13_556 ?
Sn2 Li1 2.854(11) 15_455 ?
Sn2 Li3 2.970(7) . ?
Sn2 Li3 2.970(7) 9_556 ?
Sn2 Li4 2.989(9) 1_556 ?
Sn2 Li4 2.989(9) . ?
Sn2 Li1 3.064(11) . ?
Sn2 Li1 3.064(11) 3_556 ?
Li1 Li3 2.697(15) . ?
Li1 Li1 2.84(2) 13_556 ?
Li1 Sn2 2.854(11) 13_556 ?
Li1 Li2 2.850(8) . ?
Li1 Li2 2.850(8) 1_556 ?
Li1 Li5 2.865(11) . ?
Li1 Li4 3.033(7) 13_556 ?
Li1 Li4 3.033(7) 13 ?
Li1 Sn1 3.230(8) 1_556 ?
Li2 Li4 2.814(19) . ?
Li2 Sn2 2.832(7) 1_554 ?
Li2 Li1 2.850(8) 1_554 ?
Li2 Li2 2.90(2) 3 ?
Li2 Li3 3.109(9) 1_554 ?
Li2 Li3 3.109(9) . ?
Li2 Li4 3.490(12) 13 ?
Li2 Li2 3.52(3) 13 ?
Li3 Li1 2.697(15) 11 ?
Li3 Li3 2.86(3) 9_556 ?
Li3 Sn2 2.970(7) 9_556 ?
Li3 Sn1 3.082(10) 1_556 ?
Li3 Li2 3.109(9) 11 ?
Li3 Li2 3.109(9) 1_556 ?
Li3 Li2 3.109(9) 11_556 ?
Li3 Li5 3.475(15) . ?
Li4 Li2 2.814(19) 3 ?
Li4 Sn1 2.909(12) 13 ?
Li4 Sn1 2.909(12) 5_455 ?
Li4 Sn2 2.989(9) 1_554 ?
Li4 Li1 3.033(7) 13_556 ?
Li4 Li1 3.033(7) 15_454 ?
Li4 Li1 3.033(7) 13 ?
Li4 Li1 3.033(7) 15_455 ?
Li4 Li5 3.436(11) 5_455 ?
Li4 Li5 3.436(11) 5_454 ?
Li5 Sn1 2.7980(3) 9_656 ?
Li5 Sn1 2.7980(3) 9_655 ?
Li5 Sn1 2.7980(3) 1_556 ?
Li5 Li1 2.865(11) 11 ?
Li5 Li1 2.865(11) 3_656 ?
Li5 Li1 2.865(11) 9_656 ?
Li5 Li4 3.436(11) 13_556 ?
Li5 Li4 3.436(11) 5_545 ?
Li5 Li4 3.436(11) 13 ?
Li5 Li4 3.436(11) 5_546 ?
